1

**Classifying superconductivity in an infinite-layer nickelate Nd0.8Sr0.2NiO2 **

E. F. Talantsev1,2*_{ }

1_{M.N. Mikheev Institute of Metal Physics, Ural Branch, Russian Academy of Sciences, }

18, S. Kovalevskoy St., Ekaterinburg, 620108, Russia

2_{NANOTECH Centre, Ural Federal University, 19 Mira St., Ekaterinburg, 620002, }

Russia

*_{E-mail: evgeny.talantsev@imp.uran.ru }

**Abstract **

Recently Li et al (2019 Nature **572** 624) discovered a new type of oxide superconductor
Nd0.8Sr0.2NiO2 with Tc = 14 K. To classify superconductivity in this infinite-layer nickelate

experimental upper critical field, Bc2(T), and the self-field critical current densities, Jc(sf,T),

reported by Li et al (2019 Nature **572** 624), are analysed in assumption of s-, d-, and p-wave
pairing symmetries and single- and multiple-band superconductivity. Based on deduced the
ground-state superconducting energy gap, (0), the London penetration depth, (0), the

relative jump in electronic specific heat at Tc, ΔC/C, and the ratio of 2(0)/kB*T*c, we conclude

that Nd0.8Sr0.2NiO2 is type-II high- weak-coupled single-band s-wave superconductor.

2

**Classifying superconductivity in an infinite-layer nickelate Nd0.8Sr0.2NiO2 **

**I. Introduction **

For several decades the term of infinite-layer superconductor was referred to a copper-oxide superconducting compounds, Sr1−xMxCuO2 (M=La, Nd, Ca, Sr…) [1,2], until

recently, Li et al [3] have extended this class of unconventional superconductors by the discovery of superconductivity at Tc = 14 K in Nd0.8Sr0.2NiO2 nickelate. Thus, bulk

superconducting oxides family, i.e. tungsten bronzes [4], titanates [5], bismuthates [6], cuprates [7], and ruthenates [8] extends by a new nickelate member. Several research groups proposed different models for superconducting state in this compound [9-12], and the exhibiting of the superconducting state in this compound is in a debate [13].

In this paper, to classify superconductivity in this new class of oxide superconductors the
temperature-dependent upper critical field, *B*c2(T), and the self-field critical current density,

*J*c(sf,T), are analysed within s-, d-, and p-pairing symmetries. In result, it is shown that

infinite-layer Nd0.8Sr0.2NiO2 nickelate is weak-coupled single band s-wave superconductor.

**II. Models description **

The Ginzburg-Landau theory [14] has two fundamental lengths, one is the coherence length, (T), and the second is London penetration depth, (T). The ground state coherence

length, (0), is given by [14,15]:

𝐵_{𝑐2}(0) = 𝜙0

2∙𝜋∙𝜉2_{(0)}, (1)

where 𝜙_{0} = 2.068 ∙ 10−15_{ Wb is magnetic flux quantum, and B}

c2(0) is the ground state upper

critical field. For temperature dependent coherence length, (T), several models were

proposed [14,15-21]. In this paper, to deduce the ground state coherence length, (0), in

infinite-layer Nd0.8Sr0.2NiO2 nickelate superconductor, three models are used. The first model

3

𝐵_{𝑐2}(𝑇) = 𝜙0
2∙𝜋∙𝜉2_{(0)}∙ (

1.77−0.43∙(𝑇 𝑇𝑐)

2

+0.07∙(𝑇 𝑇𝑐)

4

1.77 ) ∙ [1 − (

𝑇 𝑇𝑐)

2

]. (2)

The second model was proposed by Baumgartner et al [20] (B-WHH):

𝐵_{𝑐2}(𝑇) = 𝜙0
2∙𝜋∙𝜉2_{(0)}∙ (

(1−𝑇

𝑇𝑐)−0.153∙(1− 𝑇 𝑇𝑐)

2

−0.152∙(1−𝑇 𝑇𝑐)

4

0.693 ) (3)

And the third model was proposed recently in our recent report [21]:

𝐵_{𝑐2}(𝑇) = 𝜙0
2∙𝜋∙𝜉2_{(0)}∙

[

(1.77−0.43∙( 𝑇 𝑇𝑐)

2

+0.07∙(𝑇 𝑇𝑐)

4

1.77 )

2

∙ 1

1− 1 2∙𝑘𝐵∙𝑇∙∫

𝑑𝜀

𝑐𝑜𝑠ℎ2(√𝜀2+Δ2(𝑇) 2∙𝑘𝐵∙𝑇 ) ∞

0

]

(4)

where kB is Boltzmann constant, and (T) is the temperature-dependent superconducting gap,

for which analytical expression was given by Gross et al [22]:

Δ(𝑇) = Δ(0) ∙ 𝑡𝑎𝑛ℎ [𝜋∙𝑘𝐵∙𝑇𝑐 Δ(0) ∙ √𝜂 ∙

Δ𝐶 𝐶 ∙ (

𝑇𝑐

𝑇 − 1)] (5)

where (0) is the ground state energy gap amplitude, ΔC/C is the relative jump in electronic

specific heat at Tc, = 2/3 for s-wave superconductors [22].

Thus, (0) and Tc can be obtained by fitting experimental Bc2(T) data to Eqs. 2-4. In

addition, C/C, (0) and, thus, the ratio of 2Δ(0)

𝑘𝐵𝑇𝑐 , can be deduced as free-fitting parameters by

fitting experimental Bc2(T) data to Eq. 4. More details about the procedures can be found

elsewhere [23].

There is an alternative way to deduce (0), C/C, Tc and 2Δ(0)

𝑘𝐵𝑇𝑐 by the fit of experimental

self-field critical current density, Jc(sf,T), to universal equation, which is for thin-film

superconductors reduced to simple form [23,24]:

𝐽_{𝑐}(sf, 𝑇) = 𝜙0
4𝜋𝜇0∙

𝑙𝑛(1+√2∙𝜆(0)_{𝜉(0)})

𝜆3_{(𝑇)} (6)

where ϕ0 = 2.067 × 10−15 Wb is the magnetic flux quantum, *µ*0 = 4π × 10−7 H/m is the

4

1. 𝜆(𝑇) = 𝜆(0)

√1− 1 2∙𝑘𝐵∙𝑇∙∫

𝑑𝜀

cosh2(√𝜀2+Δ2(𝑇) 2∙𝑘𝐵∙𝑇 ) ∞

0

, (7)

for s-wave superconductors, where (T) is given by Eq. 5 [22,25].

2. 𝜆(𝑇) = 𝜆(0)

√1− 1

2∙𝑘𝐵∙𝑇∙∫ 𝑐𝑜𝑠
2_{(𝜃)∙}
2𝜋

0 (∫

𝑑𝜀

𝑐𝑜𝑠ℎ2(√𝜀2+Δ2(𝑇,𝜃) 2∙𝑘𝐵∙𝑇 ) ∞

0 )∙𝑑𝜃

(8)

for d-wave superconductors, where the superconducting energy gap, (T,), is given by

[22,25]:

Δ(𝑇, 𝜃) = Δ_{𝑚}(𝑇) ∙ 𝑐𝑜𝑠(2𝜃) (9)

where m(T) is the is the maximum amplitude of the k-dependent d-wave gap given by Eq. 5,

is the angle around the Fermi surface subtended at (, ) in the Brillouin zone (details can

be found elsewhere [22,25,26]). In Eq. 9 the value of = 7/5 [22,25,26].

3. And p-wave symmetry [22,25], which only recently was tested to fit critical current densities in superconductors [22,25]:

𝜆_{(𝑝,𝑎)(⊥,∥)}(𝑇) = 𝜆(𝑝,𝑎)(⊥,∥)(0)

√ 1− 3

4∙𝑘𝐵∙𝑇∙∫ 𝑤⊥,∥(𝑥)∙ 1 0

(

∫ 𝑑𝜀

𝑐𝑜𝑠ℎ2

(

√𝜀2+Δ𝑝,𝑎2 (𝑇)∙𝑓𝑝,𝑎2 (𝑥) 2∙𝑘𝐵∙𝑇

) ∞

0

) ∙𝑑𝑥

(10)

where subscripts p, a, ⊥, and ∥ designate polar, axial, perpendicular and parallel cases respectively. For this symmetry, the gap function is given by [22,25]:

### Δ

### (𝒌

### ̂, 𝑇) =

### Δ

### (𝑇)𝑓(𝒌

### ̂, 𝒍̂)

(11)where, (T) is the superconducting gap amplitude, * k* is the wave vector, and

*is the gap axis.*

**l**Thus, temperature dependence of (T) is determined by mutual orientation of the vector

5
There are two distinctive orientations, **A*** l* (when

*is perpendicular to*

**A***) and polar*

**l****A**

**l**(when * A* is parallel to

*) [22,25]. More details can be found elsewhere [22,25,26]). The function of 𝑤⊥,∥(𝑥) in Eq. 10 is:*

**l**𝑤_{⊥}(𝑥) = (1 − 𝑥2_{)/2}_{ } _{ (12) }

and

𝑤_{∥}(𝑥) = 𝑥2_{ } _{ (13) }

and the gap amplitude in Eq. 11 is just Eq. 5, but is given by [25]:

η_{𝑝,𝑎} =2
3∙

1

∫ 𝑓𝑝,𝑎2 1

0 (𝑥)∙𝑑𝑥

(14)

where

𝑓_{𝑝}(𝑥) = 𝑥 ; polar configuration (15)

𝑓_{𝑎}(𝑥) = √1 − 𝑥2_{; axial configuration } _{ (16) }

More details about the Jc(sf,T) analysis for p-wave symmetry can be found elsewhere [26,27].

By substituting Eqs. 5, 7-13 in Eq. 6, one can fit experimental Jc(sf,T) data to s-, d-,

p-wave gap symmetries to deduce (0), Δ(0), ΔC/C, Tc and 2Δ(0)

𝑘𝐵𝑇𝑐 as free-fitting parameters.

This approach is recently applied for wide range of thin film unconventional superconductors [23,24,26-32].

**III. ****B****c2(****T****) analysis **

There are several criteria to define Bc2(T) from experimental R(T) curves. In this paper ti

define Bc2(T) we use the criterion of 3% of normal state resistance, Rnorm(T), for R(T) curves

of Nd0.8Sr0.2NiO2 presented in Fig. 4(a) by Li et al [3]. The fits of Bc2(T) data to three models

are shown in Fig. 1. It can be seen that (0) values deduced by three models are close to each

other and following analysis of Jc(sf,T) will be utilized an average value of:

6

**Figure 1.** The upper critical field, Bc2(T), of Nd0.8Sr0.2NiO2 (reported by Li et al [3]) and data

fits to three models (Eqs. 2-4). (a) fit to Gor’kov model, the fit quality is R = 0.995. (b) fit to B-WHH, R = 0.998. (c) fit to Eq. 4, R = 0.9993. 95% confidence bars are shown.

0 2 4 6 8 10 12 0 2 4 6 8 10

0 2 4 6 8 10 12

0 2 4 6 8 10

**c**

**b**

*B*_{c2}(*T*)

Gor'kov model fit

m ag ne ti c f lux d en s ity ( T

)

**Nd**

**0.8**

**Sr**

**0.2**

**NiO**

**2**

*T*_{c} = 10.9 ± 0.1 K
(0) = 5.8 ± 0.1 nm

**a**

*B*_{c2}(*T*)

B-WHH fit m ag ne ti c f lux d en s ity ( T )

*T*_{c} = 10.9 ± 0.1 K
(0) = 5.6 ± 0.1 nm

*C*/*C* = 1.5 ± 0.2
(0) = 1.65 ± 0.09 meV
2(0)/*k*_{B}*T*_{c} = 3.5 ± 0.3

*B*_{c2}(*T*)

fit to Eq. 4

m ag ne ti c f lux d en s ity ( T ) temperature (K)

7 This deduced value for (0) is in reasonable agreement with (0) = 4.5 nm reported by

Jovanović et al. [33] for copper-oxide-based infinite layer counterpart of La1-xSrxCuO2.

Deduced values by the fit to Eq. 4:

2Δ(0)

𝑘𝐵𝑇𝑐 = 3.5 ± 0.3 (18)

ΔC

𝐶 = 1.5 ± 0.2 (19)

are, within uncertainties, equal to BCS [34] weak-coupling limits of 3.53 and 1.43 respectively, and the former deduced value is equal to recently deduced value of:

2Δ(0)

𝑘𝐵𝑇𝑐 = 3.51 ± 0.05 (20)

for s-wave oxide superconductor of Ba0.51K0.49BiO3 [35].

It should be noted that there is no sign in experimental *B*c2(*T*) data that Nd0.8Sr0.2NiO2
exhibits two superconducting band state, which can be seen as sharp enhancement in

amplitude of *B*c2(*T*) at critical temperature of the second superconducting band opening (see

for details Ref. 36).

**IV. ****J****c(sf,****T****) analysis **

The critical current density, Jc, is defined as the lowest, detectable in experiment, value of

electric power dissipation in a superconductor on electric current flow. For available E(I) curves presented by Li et al [3] in their Fig. 3(f), the critical current density at self-field condition (when no external magnetic field is applied), Jc(sf,T), can be defined at the lowest

value of electric field of Ec = 3 V/cm. Experimental Jc(sf,T) deduced by this Ec criterion and

the fit to single band s-wave model (i.e., Eqs. 6,7 for which (0) = 5.7 nm was fixed) are

8

**Figure 2.** The self-field critical current density, Jc(sf,T), for Nd0.8Sr0.2NiO2 thin film with raw

data processed from the work of Li et al. [3] and a fit of the data to three single-band models. For all models (0) = 5.7 nm was used. (a) s-wave fit, (0) = 740 ± 3 nm, Tc = 12.2 ± 0.1 K,

the goodness of fit R = 0.995; (b) p-wave axial **A*** l* fit, (0) = 738 ± 2 nm, Tc = 12.3 ± 0.1 K,

*R = 0.997; (c) p-wave polar ***A*** l* fit, (0) = 735 ± 2 nm, Tc = 12.4 ± 0.1 K R = 0.9990. Other

deduced parameters are listed in Table I. 0.00 0.06 0.12 0.18 0.24 0.00 0.06 0.12 0.18

0 2 4 6 8 10 12

0.00 0.06 0.12 0.18

**b**

fit to *s*-wave

= 130

*J*_{c}(sf,*T*)
(*T*)

critical current density (MA/cm

2 ) **Nd _{0.8}Sr_{0.2}NiO_{2}**

**J**

**J**

_{c}2(0)/*k*_{B}*T*_{c} = 3.5 ± 0.1

**a**
0.6
0.9
1.2
1.5
1.8
2.1

###

London penetration depth (

m)

fit to axial A**l **

*J*_{c}(sf,*T*)
(*T*)

c ri ti c a l c u rr e n t d e n s it y ( M A /c m 2 )

**J**

**J**

_{c}2(0)/*k*_{B}*T*_{c} = 4.1 ± 0.1

0.6 0.9 1.2 1.5 1.8

###

L o n d o n p e n e tr a ti o n d e p th ( m)**c**

*J*_{c}(sf,*T*)
(*T*)

fit to polar A||**l**

c ri ti c a l c u rr e n t d e n s it y ( M A /c m 2 ) temperature (K)

**J**

**J**

_{c}2(0)/*k*_{B}*T*_{c} = 5.3 ± 0.2

9 Deduced (0) = 740 ± 3 nm is similar to (0) = 690-850 nm measured for samples

possessing maximal Tc values for cuprate counterpart La1-xSrxCuO2 [37].

By utilizing deduced (0) value the Ginzburg-Landau parameter 𝜅 =λ(0)

𝜉(0) = 130 which is

similar to La1-xSrxCuO2 [33,37] and this value is at the upper-level range for other cuprates

and unconventional superconductors [15,23,24,26,38-43].

**Table I.** Deduced 2Δ(0)/kB*T*c and ΔC/C values for Nd0.8Sr0.2NiO2 from Jc(sf,T) fits to Eqs.

6-8 and BCS weak-coupling limits for the same parameters within for s-, d-, and p-wave pairing symmetries [20,23]. For d-wave symmetry, Δ𝑚(0) was used (which is the maximum

amplitude of the k-dependent d-wave gap, Δ(𝜃) = Δ𝑚(0)cos(2𝜃)).

**Pairing symmetry and **
**experiment geometry **

Deduced

2Δ(0)
𝑘_{𝐵}𝑇_{𝑐}

BCS weak-coupling limit of

2Δ(0)
𝑘_{𝐵}𝑇_{𝑐}

Deduced

Δ𝐶 𝐶

BCS weak-coupling limit of

Δ𝐶 𝐶

*s-wave * 3.5 ± 0.2 3.53 1.5 ± 0.2 1.43

*d-wave * > 102 4.28 2.3 ± 0.5 0.995

*p-wave; axial ***A*** l* 4.1 ± 0.1 4.06 1.07 ± 0.08 1.19

*p-wave; axial ***A*** l* 9.0 ± 2.4 4.06 1.55 ± 0.05 1.19

*p-wave; polar ***A*** l* > 5·102 4.92 2.5 ± 0.4 0.79

*p-wave; polar ***A*** l* 5.3 ± 0.3 4.92 0.63 ± 0.03 0.79

Alternatively, d- and p-wave superconducting gap symmetries can be considered. The fits

to d-wave symmetry, as well as to polar **A*** l* and axial

**A**

*of p-wave, reveal very large 2Δ(0)*

**l**𝑘𝐵𝑇𝑐

values and these symmetries can be excluded from further consideration.

The cases of polar **A*** l* and axial

**A**

*gap symmetries are still hypothetically possible*

**l**10 given experimental conditions (i.e. epitaxial c-axis oriented thin film) expected geometry is

polar **A*** l* [21].

It should be also noted that there is no sign for two-band superconductivity in

Nd0.8Sr0.2NiO2 which usually can be detected by a sharp enhancement in Jc(sf,T) at critical

temperature of the second band opening [24,36].

By taking in account a good agreement between 2Δ(0)

𝑘𝐵𝑇𝑐 and Δ𝐶

𝐶 values deduced for s-wave

symmetry from Bc2(T) and Jc(sf,T) analyses (Eqs. 17, 18 and Table 1, respectively), which

are, in addition, within BCS weak-coupling limits for this symmetry, and a fact that s-wave pairing symmetry is the most conventional one, we can conclude that Nd0.8Sr0.2NiO2

nickelate is weak-coupling single band high- s-wave superconductor.

**V. Conclusions **

Recently discovered [3] an infinite-layer nickelate Nd0.8Sr0.2NiO2 superconductor is a new

member of bulk oxide superconductors for which experimental Bc2(T) and Jc(sf,T) data are

analysed in this paper.

In result, it is found that an infinite-layer nickelate Nd0.8Sr0.2NiO2 is weak-coupling single

band high- s-wave superconductor.

**Acknowledgement **

11 Author also thanks financial support provided by the state assignment of Minobrnauki of Russia (theme “Pressure” No. АААА-А18-118020190104-3) and by Act 211 Government of

the Russian Federation, contract No. 02.A03.21.0006.

**References **

[1] Siegrist T, Zahurak S M, Murphy D W and Roth R S 1988 The parent structure of the
layered high-temperature superconductors 1988 Nature **334** 231–232

[2] Azuma M, Hiroi Z, Takano M, Bando Y and Takeda Y 1992 Superconductivity at 110 K
in the infinite-layer compound (Sr1-xCax)1-yCuO2 Nature **356** 775-776

[3] Li D, Lee K, Wang B Y, Osada M, Crossley S, Lee H R, Cui Y, Hikita Y and Hwang H
Y 2019 Superconductivity in an infinite-layer nickelate Nature **572** 624-627

[4] Remeika J P, Geballe T H, Matthias B T, Cooper A S, Hull G W, Kelly E M 1967
Superconductivity in hexagonal tungsten bronzes Physics Letters A **24** 565-566

[5] Johnston D C, Prakash H, Zachariasen W H, Viswanathan R 1973 High temperature
superconductivity in the LiTiO ternary system Materials Research Bulletin **8** 777-784
[6] Sleight A W, Gillson J L, Bierstedt P E 1975 High-temperature superconductivity in the
BaPb1-xBixO3 systems Solid State Communications **17** 27-28

[7] Bednorz J G and Müller K A 1986 Possible high Tc superconductivity in the Ba – La –
Cu – O system Zeitschrift für Physik B Condensed Matter **64** 189-193

[8] Maeno Y, Hashimoto H, Yoshida K, Nishizaki S, Fujita T, Bednorz J G and Lichtenberg
F 1994 Superconductivity in a layered perovskite without copper Nature **372** 532-534
[9] Hirsch J E, Marsiglio F 2019 Hole superconductivity in infinite-layer nickelates Physica
*C ***566** 1353534

[10] Botana A S, Norman M R 2019 Similarities and differences between infinite-layer nickelates and cuprates and implications for superconductivity arXiv:1908.10946v2 [11] Jiang M, Berciu M, Sawatzky G A 2019 Doped holes in NdNiO2 and high-Tc cuprates

show little similarity arXiv:1909.02557

[12] Nomura Y, et al 2019 Formation of a two-dimensional single-component correlated
electron system and band engineering in the nickelate superconductor NdNiO2 Phys. Rev. B
**100** 205138

[13] Li Q, He C, Si J, Zhu X, Zhang Y, Wen H-H 2019 Absence of superconductivity in bulk Nd1−xSrxNiO2 arXiv:1911.02420v3

[14] Ginzburg V L and Landau L D 1950 On the theory of superconductivity Zh. Eksp. Teor.
*Fiz. ***20** 1064-1082

[15] Poole P P, Farach H A, Creswick R J, Prozorov R 2007 Superconductivity (2-nd Edition, London, UK)

[16] Gor'kov L P 1960 The critical supercooling field in superconductivity theory Soviet
*Physics JETP ***10** 593-599

[17] Jones C K, Hulm J K, Chandrasekhar B S 1964 Upper critical field of solid solution
alloys of the transition elements Rev. Mod. Phys. **36** 74-76

[18] Helfand E and Werthamer N R 1966 Temperature and purity dependence of the
superconducting critical field, Hc2. II. Phys. Rev. **147** 288-294

[19] Werthamer N R, Helfand E and Hohenberg P C 1966 Temperature and purity

dependence of the superconducting critical field, Hc2. III. Electron spin and spin-orbit effects

12 [20] Baumgartner T, Eisterer M, Weber H W, Fluekiger R, Scheuerlein C, Bottura L 2014 Effects of neutron irradiation on pinning force scaling in state-of-the-art Nb3Sn wires

*Supercond. Sci. Technol. ***27** 015005

[21] Talantsev E F 2019 Classifying superconductivity in compressed H3S Modern Physics

*Letters B ***33** 1950195

[22] Gross F, Chandrasekhar B S, Einzel D, Andres K, Hirschfeld P J, Ott H R, Beuers J,
Fisk Z, Smith J L 1986 Anomalous temperature dependence of the magnetic field penetration
depth in superconducting UBe3 Z. Phys. B - Condensed Matter **64** 175-188

[23] Talantsev E F 2018 Critical de Broglie wavelength in superconductors Modern Physics
*Letters B ***32** 1850114

[24] Talantsev E F, Crump W P, Island J O, Xing Y, Sun Y, Wang J, Tallon J L 2017 On the
origin of critical temperature enhancement in atomically thin superconductors 2D Materials **4**

025072

[25] Gross-Alltag F, Chandrasekhar B S, Einzel D, Hirschfeld P J, Andres K 1991 London
field penetration in heavy fermion superconductors Z. Phys. B - Condensed Matter **82**
243-255

[26] Talantsev E F, Iida K, Ohmura T, Matsumoto T, Crump W P, Strickland N M,
Wimbush S C and Ikuta H 2019 P-wave superconductivity in iron-based superconductors
*Scientific Reports ***9** 14245

[27] Talantsev E F, Mataira R C, Crump W P 2019 Classifying superconductivity in
Classifying superconductivity in Moiré graphene superlattices arXiv:1902.07410v3
[28] Fête A, Rossi L, Augieri A and Senatore C 2016 Ionic liquid gating of ultra-thin
YBa2Cu3O7-x films Applied Physics Letters **109** 192601

[29] Liu C, et al. 2018 Two-dimensional superconductivity and topological states in PdTe2

thin films Phys. Rev. Materials **2** 094001

[30] Qu D-X, Teslich N E, Dai Z, Chapline G F, Schenkel T, Durham S R and Dubois J
2018 Onset of a two-dimensional superconducting phase in a
topological-insulator–normal-metal Bi1-xSbx/Pt junction fabricated by ion-beam techniques Phys. Rev. Lett. **121** 037001

[31] Pal B, et al. 2019 Experimental evidence of a very thin superconducting layer in
epitaxial indium nitride Supercond. Sci. Technol. **32** 015009

[32] Zheliuk O, Lu J M, Chen Q H, El Yumin A A, Golightly S and Ye J T 2019 Josephson coupled Ising pairing induced in suspended MoS2 bilayers by double-side ionic gating Nature

*Nanotechnology ***14**1123-1128

[33] Jovanović V P, Li Z Z, Raffy H, Briatico J, Sinchenko A A, Monceau P 2009 Resistive
upper critical fields and anisotropy of an electron-doped infinite-layer cuprate *Physical *
*Review B***80** 024501

[34] Bardeen J, Cooper L N, Schrieffer J R 1957 Theory of superconductivity Phys. Rev. **108**

1175-1204

[35] Wen C H P, *et al.* 2018 Unveiling the superconducting mechanism of Ba0.51K0.49BiO3

*Physical Review Letters***121** 117002

[36] Talantsev E F 2019 Classifying induced superconductivity in atomically thin Dirac-cone
materials Condensed Matter **4** 83

[37] Fruchter L, Jovanovic V, Raffy H, Labdi Sid, Bouquet F and Li Z Z 2010 Penetration
depth of electron-doped infinite-layer Sr0.88La0.12CuO2+x thin films *Physical Review B***82**
144529

[38] Puźniak R, Usami R, Isawa K, and Yamauchi H 1995 Superconducting-state

thermodynamic parameters and anisotropy of HgBa2Can−1CunOy by reversible magnetization

13
[39] Hosono H et. al. 2015 Exploration of new superconductors and functional materials,
and fabrication of superconducting tapes and wires of iron pnictides Sci. Technol. Adv.
*Mater. ***16** 033503

[40] Iida K, Hänisch J, and Tarantini C 2018 Fe-based superconducting thin films on

metallic substrates: Growth, characteristics, and relevant properties Applied Physics Reviews

**5** 031304

[41] Kauffmann-Weiss S et al. 2019 Microscopic origin of highly enhanced current carrying
capabilities of thin NdFeAs(O,F) films Nanoscale Advances **1** 147

https://doi.org/10.1039/C9NA00147F

[42] Hänisch J et al. 2019 Fe-based superconducting thin films – Preparation and tuning of
superconducting properties Supercond. Sci. Technol. **32** 093001